FATIGUE TESTS AND STRESSLIFE (SN) APPROACH


 Simon Kory Singleton
 2 years ago
 Views:
Transcription
1 FATIGUE TESTS AND STRESSLIFE (SN) APPROACH FATIGUE TESTING LOADING TEST MACHINES SPECIMENS STANDARDS STRESSLIFE APPEROACH SN CURVES MEAN STRESS EFFECTS ON SN BEHAVIOR FACTORS INFLUENCING SN BEHAVIOR SN CURVE REPRESENTATION AND APPROXIMATIONS EXAMPLE OF LIFE ESTIMATION USING SN APPROACH Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 1
2 FATIGUE LOADING Some load histories may be simple and repetitive, while in other cases they may be completely random. The randomness may contain substantial portions of more deterministic loading. For example, the groundairground cycle of an aircraft has substantial similarity from flight to flight. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 2
3 GroundAirGround Cycle Of An Aircraft Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 3
4 Typical Load Histories From Actual Ground Vehicle Components Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 4
5 A Typical Load History of ShortSpan Bridge Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 5
6 FATIGUE LOADING (CONTINUED) These load histories are typical of those found in reallife engineering situations. Fatigue from variable amplitude loading involving histories such as these is discussed in Chapter 9. Constant amplitude loading is introduced in this chapter. Constant amplitude loading is used: To obtain material fatigue behavior/properties for use in fatigue design, Some reallife load histories can occasionally be modeled as essentially constant amplitude. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 6
7 CONSTANT AMPLITUDE LOADING Minimum stress, S min Maximum stress, S max Stress range, S Alternating stress, S a Mean stress, S m Stress ratio, R Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 7
8 FATIGUE LOADING (CONTINUED) S a S 2 S max S min 2 S m S max S min 2 R S S min max S S max min S m S a S m S a A S S a m Stresses can be replaced with load, moment, torque, strain, deflection, or stress intensity factors. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 8
9 FATIGUE LOADING (CONTINUED) R = 1 and R = 0 are two common reference test conditions used for obtaining fatigue properties. R = 1 is called the fully reversed condition since S min = S max R = 0, where S min = 0, is called pulsating tension. One cycle is the smallest segment of the stress versus time history which is repeated periodically. Under variable amplitude loading, the definition of one cycle is not clear and hence reversals of stress are often considered. In constant amplitude loading, one cycle equals two reversals. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 9
10 FATIGUE LOADING (CONTINUED) Tensile and/or compressive mean loads and fully reversed loads are prevalent in all fields of engineering. Examples of different mean loadings. The transmission history indicates significant tensile mean stress. The suspension history shows significant compressive mean stress loading. The bracket history is dominated by essentially fully reversed, R = 1, loading. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 10
11 FATIGUE LOADING (CONTINUED) A thin or thickwalled pressure vessel subjected to cyclic internal pressure represents a component subjected to mean tensile stresses. Helical compression springs are actually under torsion, but the applied cyclic forces involve compressive mean forces. A cantilever beam deflected at the free end and then released to vibrate represents a damped vibration with essentially zero mean stress. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 11
12 FATIGUE TEST MACHINES Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 12
13 Rotating Cantilever Bending Fatigue Test Machine Constant load amplitude Nonuniform bending moment along the specimen length Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 13
14 Rotating Bending Test Machine Constant load amplitude Uniform bending moment along the specimen length Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 14
15 Constant Deflection Amplitude Cantilever Bending Test Machine Load amplitude changes with specimen cyclic hardening or softening and decreases as cracks in the specimen nucleate and grow. The eccentric crank test machines do have an advantage over the rotating bending test machines in that the mean deflection, and hence the initial mean stress, can be varied. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 15
16 Schematic of an Axial Loaded Fatigue Test Machine Capable of applying both mean and alternating axial loads in tension and/or compression Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 16
17 A Test Setup For Combined Inphase Torsion and Bending With or Without Mean Stress Uniform torque and a nonuniform bending moment along the specimen length Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 17
18 A Modern Servohydraulic Test System Principle of operation includes: generating an input signal of load, strain, or displacement using a function generator, applying this input through a hydraulic actuator, measure the specimen response via a load cell, clip gage, or an LVDT, compare this output with the input. The difference drives the system. Control and test data outputs are usually through a PC and software. Test frequency can range from mhz to khz. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 18
19 A Modern Servohydraulic Test System These test systems can perform: constant or variable amplitude load, strain, deformation, or stress intensity factor controlled tests on small specimens or can be utilized with hydraulic jacks for components, subassemblies, or whole structures. Two or more control systems are used for multiaxial testing. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 19
20 COMMON FATIGUE TEST SPECIMENS (a) Rotating bending, (b) Axial uniform, (c) Axial hourglass These specimens are usually used for axial or bending tests. These specimens usually have finely polished surfaces to minimize surface roughness effects. No distinction between crack nucleation and growth is normally made with these specimens. Careful alignment is needed for axial loaded specimens to minimize bending. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 20
21 COMMON FATIGUE TEST SPECIMENS (Axial or bending with circumferential groove) Stress concentration influence can be studied with most of these specimens by machining in notches, holes, or grooves. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 21
22 COMMON FATIGUE TEST SPECIMENS A thinwalled tube specimen designed for torsion and combined axial/torsion with the possibility of adding internal and/or external pressure. This multiaxial loading can be performed inphase or outofphase. The thinwalled tube allows for essentially uniform normal and shear stresses in the crosssectional area. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 22
23 Cantilever Flat Sheet Specimen Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 23
24 COMMON FATIGUE TEST SPECIMENS Specimens shown have been used for obtaining fatigue crack growth data. In all cases a thin slit, notch, or groove with a very small root radius is machined into the specimen. Fatigue crack growth testing is covered in Section 6.4. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 24
25 ASTM Standard Practices Related to Fatigue Testing of Metals E466 E467 E468 E606 Conducting Force Controlled Constant Amplitude Axial Fatigue Tests of Metallic Materials. Verification of Constant Amplitude Dynamic Forces in an Axial Fatigue Testing System. Presentation of Constant Amplitude Fatigue Test Results for Metallic Materials. StrainControlled Fatigue Testing. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 25
26 ASTM Standard Practices Related to Fatigue Testing of Metals (Continued) E647 Measurement of Fatigue Crack Growth Rates. E739 Statistical Analysis of Linear or Linearized StressLife (SN) and StrainLife ( N) Fatigue Data. E1012 Verification of Specimen Alignment Under Tensile Loading E1049 Cycle Counting in Fatigue Analysis. E1823 Standard Terminology Relating to Fatigue and Fracture Testing. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 26
27 ISO Standards Related to Fatigue Testing of Metals ISO/DIS Metallic MaterialsFatigue Testing Axial StrainControlled Method. ISO/DIS Metallic MaterialsFatigue Testing Statistical Planning and Analysis of Data. ISO/DIS Metallic MaterialsFatigue Testing Fatigue Crack Growth Method. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 27
28 STRESSLIFE (SN) APPROACH SN CURVES MEAN STRESS EFFECTS ON SN BEHAVIOR FACTORS INFLUENCING SN BEHAVIOR SN CURVE REPRESENTATION AND APPROXIMATIONS EXAMPLE OF LIFE ESTIMATION USING SN APPROACH Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 28
29 STRESSLIFE CURVES, SN Typical schematic SN curve obtained under axial load or stress control test conditions with smooth specimens. Constant amplitude SN curves of this type are plotted on semilog or loglog coordinates. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 29
30 STRESSLIFE CURVES, SN SN curves obtained under torsion or bending loadcontrol test conditions often do not have data at the shorter fatigue lives (say 10 3 or 10 4 cycles and less) due to significant plastic deformation. Torsion and bending stress equations = T r / J and = M y / I can only be used for nominal elastic behavior. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 30
31 STRESSLIFE CURVES, SN (Continued) Typical variability with less variability at shorter lives and greater variability at longer lives. Variability in life for a given stress level can range from less than a factor of two to more than an order of magnitude. Variability and statistical aspects of fatigue data are discussed in Ch. 13. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 31
32 STRESSLIFE CURVES, SN (Continued) Fig. (a) shows a continuous sloping curve, while Fig. (b) shows a discontinuity or knee in the SN curve. This knee has been found in only a few materials (i.e. low and medium strength steels) between 10 6 and 10 7 cycles in noncorrosive conditions. Most materials do not contain the knee even under controlled environments. Under corrosive environments all SN data have a continuous sloping curve. When sufficient data are available, SN curves are usually drawn through median points and thus represent 50 percent expected failures. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 32
33 STRESSLIFE CURVES, SN (Continued) Common terms used with the SN diagram are Fatigue life, N : f The number of cycles of stress or strain that a specimen sustains before failure occurs. Fatigue strength: A hypothetical value of stress at failure for exactly N f cycles as determined from an SN diagram. Fatigue limit, S : f The limiting value of the median fatigue strength as N f becomes very large. Endurance limit is often implied as being analogous to the fatigue limit. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 33
34 STRESSLIFE CURVES, SN (Continued) Fatigue typically consists of crack nucleation, growth, and final fracture, as it was emphasized in Chapter 3. A reasonable crack nucleation life can be defined by a crack length of 0.25mm (0.01in.). This dimension can relate to engineering dimensions and can represent a small macrocrack. The number of cycles to form this small crack in smooth unnotched or notched fatigue specimens and components can range from a few percent to almost the entire life, as illustrated schematically. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 34
35 STRESSLIFE CURVES, SN (Continued) A larger fraction of life for crack growth, the shaded area, occurs at higher stress levels, while a larger fraction of life for crack nucleation occurs at lower stress levels. When fatigue crack growth life is significant, then fracture mechanics, as discussed in Chapter 6, should be used. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 35
36 STRESSLIFE CURVES, SN (Continued) The fatigue limit has historically been a prime consideration for longlife fatigue design. For a given material the fatigue limit has an enormous range depending on: surface finish, size, type of loading, temperature, corrosive, and other aggressive environments, mean stresses, residual stresses, and stress concentrations. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 36
37 STRESSLIFE CURVES, SN (Continued) Fatigue limit based on a nominal alternating stress, S a : Can range from essentially 1 to 70 percent of the ultimate tensile strength. Example of a case where the fatigue limit may be approximately 1 percent of S u is a high strength steel with a sharp notch subjected to a high mean tensile stress in a very corrosive atmosphere. An example of a case when the fatigue limit might approach 70 percent of S u is a medium strength steel in an inert atmosphere containing appreciable compressive residual stresses. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 37
38 STRESSLIFE CURVES, SN (Continued) Most longlife SN fatigue data available in the literature consist of fully reversed (S m = 0) uniaxial fatigue strengths or fatigue limits of small highly polished unnotched specimens based on 10 6 to 5 x 10 8 cycles to failure in laboratory air environment. Representative monotonic tensile properties and bending fatigue limits of selected engineering alloys obtained under the above conditions are given in Table A.1. The fatigue limits given in Table A.1 must be substantially reduced in most cases before they can be used in design situations. For example, 10 to 25 percent reductions in these values for just size effect alone is not unreasonable for bend specimens greater than 10 mm (0.4 in.) in diameter. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 38
39 Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 39
40 Rotating Bending Fatigue Limits or Fatigue Strengths Based on 10 7 to 10 8 Cycles for Steels Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 40
41 Rotating Bending Fatigue Limits or Fatigue Strengths Based on 10 7 Cycles for Irons O nodular cast iron ingot iron + malleable cast iron * wrought iron Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 41
42 Rotating Bending Fatigue Limits or Fatigue Strengths Based on 10 8 Cycles for Aluminum Alloys * cast x wrought Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 42
43 Rotating Bending Fatigue Limits or Fatigue Strengths for Wrought Copper Alloys Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 43
44 STRESSLIFE CURVES, SN (Continued) S f /S u varies from about 0.25 to 0.65 for these data. There is a tendency to generalize that S f increases linearly with S u. These figures show this is incorrect and data bands tend to bend over at the higher ultimate strengths. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 44
45 STRESSLIFE CURVES, SN (Continued) For steels, substantial data are clustered near fatigue ratio S f /S u 0.5 for the low and medium strength steels. The data actually fall between 0.35 and 0.6 for S u < 1400 MPa (200 ksi). For S u > 1400 MPa (200 ksi), S f does not increase significantly. Common estimates for unnotched, highly polished, small bending specimen fatigue limits for steels are: S f = 0.5 S u S f = 700 MPa for S u 1400 MPa (200 ksi) for S u 1400 MPa (200 ksi) For steels, S u can be approximated from the Brinell hardness, HB, as: S u = 3.45HB for MPa units S u = 0.5HB for ksi units Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 45
46 STRESSLIFE CURVES, SN (Continued) These equations are not unreasonable for small highly polished steel specimens, but empirical reduction factors for surface finish, size, stress concentration, temperature, and corrosion must also be considered. We strongly warn against using a design fatigue limit equal to onehalf the ultimate strength for steels. Most data in Fig. 4.8 for irons, aluminum, and copper alloys fall below the 0.5 fatigue ratio. The aluminum and copper alloy data bands bend over at higher strengths as do the bands for steels. Thus high strength steels, aluminum, and copper alloys generally do not exhibit corresponding high unnotched fatigue limits. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 46
47 Schematic Scatter Bands For Steels Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 47
48 MEAN STRESS EFFECTS ON SN BEHAVIOR The mean stress, S m, can have substantial influence on fatigue behavior. In general, tensile mean stresses are detrimental and compressive mean stresses are beneficial. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 48
49 MEAN STRESS EFFECTS ON SN BEHAVIOR At intermediate or high stress levels under load control test conditions, substantial cyclic creep (also referred to as cyclic ratcheting) which increases the mean strain, can occur in the presence of mean stresses. This cyclic creep adds to the detrimental effects of tensile mean stress on fatigue life and results in additional undesirable excess deformation. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 49
50 Tensile Mean Stress Influence on Longlife (10 7 Cycles) Fatigue Strength For Steel Alloys S f is the fully reversed, (S m = 0, R = 1), fatigue limit of smooth specimens Similar behavior exists for other alloys. The general trend indicates that tensile mean stresses are detrimental. Much of the data fall between the straight and curved lines. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 50
51 Tensile Mean Stress Influence on Longlife (5x10 7 Cycles) Fatigue Strength For Aluminum Alloys Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 51
52 Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 52 MEAN STRESS EFFECTS ON SN BEHAVIOR (CONT D) The straight line is the modified Goodman line. The curve is the Gerber parabola. An additional popular relationship has been formulated by replacing S u with f (Morrow line) where f is the true fracture strength. 1 f m f a S S S 1 2 u m f a S S S S 1 u m f a S S S S
53 Compressive Mean Stress Effects for Several Steels and Aluminum Alloys These compressive mean stresses cause increases of up to 50 percent in the alternating fatigue strength. This increase is too often overlooked, since compressive residual stresses can cause similar beneficial behavior. The modified Goodman or Morrow equations can be extrapolated into the compression mean stress region. The Gerber equation incorrectly predicts a detrimental effect of compressive mean stresses. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 53
54 MEAN STRESS EFFECTS ON SN BEHAVIOR (CONT D) The modified Goodman and Morrow equations are shown for a given long life (e.g 10 7 cycles) along with the criterion for yielding: S a /S y ' + S m /S y =1 If the coordinates of the applied alternating and mean stresses fall within the modified Goodman or Morrow lines, then fatigue failure should not occur prior to the given life. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 54
55 MEAN STRESS EFFECTS ON SN BEHAVIOR (CONT D) If yielding is not to occur, then the applied alternating and mean stresses must fall within the two yield lines connecting S y to S y. If both fatigue failure and yielding are not to occur, then neither criterion, as indicated by the three bold lines should be exceeded. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 55
56 FACTORS INFLUENCING SN BEHAVIOR The reference fatigue condition for SN behavior is usually fully reversed R = 1 bending or axial loading using small unnotched specimens. In addition to mean stress many other factors also affect the reference fatigue condition. Some of these are discussed in other chapters: notches and stress concentrations (Chapter 7) residual stress and surface treatment (Chapter 8) variable amplitude loading (Chapter 9) multiaxial and torsion loading (Chapter 10) corrosion (Section 11.1) fretting (Section 11.2) low temperature (Section 11.3) high temperature (Section 11.4) Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 56
57 FACTORS INFLUENCING SN BEHAVIOR (CONT D) Additional factors that influence SN behavior are: Microstructure Size Effects Surface Finish Frequency Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 57
58 FACTORS INFLUENCING SN BEHAVIOR (MICROSTRUCTURE) Metal fatigue is significantly influenced by microstructure. Microstructure includes: chemistry, heat treatment, cold working, grain size, anisotropy, inclusions, voids/porosity, and other discontinuities or imperfections. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 58
59 FACTORS INFLUENCING SN BEHAVIOR (MICROSTRUCTURE, CONT D) If the actual SN data are available, microstructural effects are inherently accounted for and do not have to be accounted for again. Chemistry, heat treatment, and cold working have an enormous number of synergistic variations, and generalities concerning their effects on fatigue behavior can not be made. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 59
60 FACTORS INFLUENCING SN BEHAVIOR (MICROSTRUCTURE, CONT D) Some generalities for the other microstructural aspects. Fine grain size generally provides better SN fatigue resistance than coarser grains, except at elevated temperatures where creep/fatigue interaction exists. Fine grains reduce localized strains along slip bands reducing the amount of irreversible slip and provide more grain boundaries to aid in transcrystalline crack arrest and deflection, and thus reduce fatigue crack growth rates. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 60
61 FACTORS INFLUENCING SN BEHAVIOR (MICROSTRUCTURE, CONT D) Anisotropy caused by cold working gives increased SN fatigue resistance when loaded in the direction of the working than when loaded in the transverse direction. This is due to the elongated grain structure in the direction of the cold working. Inclusions, and voids/porosity act as stress concentrations and thus are common locations for microcracks to nucleate under cyclic load, or to form during heat treatment or cold working prior to cyclic loading. Minimizing inclusions, voids/porosity, and other discontinuities through carefully controlled production and manufacturing procedures is a key to good fatigue resistance. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 61
62 FACTORS INFLUENCING SN BEHAVIOR (SIZE EFFECTS) Under unnotched bending conditions if the diameter or thickness of the specimen is 10mm (0.4 in.) then the SN fatigue behavior for steels is reasonably independent of the diameter or thickness. For larger size, the SN fatigue resistance is decreased as the diameter or thickness increases to 50 mm (2 in.), the fatigue limit for steels decreases to a limiting factor of about 0.7 to 0.8 of the fatigue limit for specimens less than 10 mm (0.4 in.) in diameter or thickness. Additional decreases can occur for larger specimens or components. Under unnotched axial conditions the SN fatigue resistance is poorer than for most bending conditions. The fatigue limit for axial loading can be from 0.75 to 0.9 of the small specimen bending fatigue limits. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 62
63 FACTORS INFLUENCING SN BEHAVIOR (SIZE EFFECTS) Several factors are involved in size and axial loading effects. In bending, the larger the diameter or thickness, the smaller the bending stress gradient and hence the larger the average stress in a local region on the surface. The average stress in the local region may be the governing stress for fatigue rather than the maximum stress. For axial loaded unnotched specimens, a nominal stress gradient does not exist, and the average and maximum nominal stresses have the same magnitude resulting in less size effect than in bending. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 63
64 FACTORS INFLUENCING SN BEHAVIOR (SIZE EFFECTS) In bending and axial loading, larger specimens have a higher probability of microstructural discontinuity density in the highly stressed surface regions that contribute to the decrease in fatigue resistance. Another reason why axial fatigue resistance is lower than in bending is possible eccentricity or alignment difficulties that superimpose bending stresses on the axial stresses. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 64
65 FACTORS INFLUENCING SN BEHAVIOR (SURFACE FINISH EFFECTS) Since most fatigue failures originate at the surface, the surface will have a substantial influence on fatigue behavior. Surface effects are caused by differences in surface roughness, microstructure, chemical composition, and residual stress. This influence will be more pronounced at long lives where a greater percentage of the cycles is usually involved with crack nucleation. Reference fatigue strengths are for highly polished smooth specimens. Most engineering parts, however, are not highly polished and grinding or machining, will cause degradation in fatigue strength. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 65
66 Surface Factors, K s, as a Function of Ultimate Tensile Strength For Steels The higher the ultimate tensile strength and hardness, the greater the degradation of fatigue limits. The decreases caused from grinding and machining are more related to surface roughness and residual stresses, while hotrolled and asforged behavior include these two important aspects along with surface microstructural and chemical composition changes such as decarburization and hence surface hardenability. Avoid the hotrolled or asforged surface conditions at fatigue sensitive locations by removing the undesirable surface by grinding or machining. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 66
67 FACTORS INFLUENCING SN BEHAVIOR (FREQUENCY EFFECTS) The influence of frequency on SN behavior of metals is complicated because of synergistic effects of test temperature, corrosive environment, stressstrain sensitivity to strain rate, and frequency. Specimen heating at higher test frequency due to internal hysteresis damping can increase the specimen temperature and thus disguise the true ambient temperature fatigue behavior. Generation of heat due to cyclic loading depends on the volume of highly stressed material. Axial loading will produce more heat than bending or notched specimens. Thus, frequency effects can be different. If heating and corrosion effects are negligible, frequencies from less than 1 Hz to 200 Hz have had only a small effect on SN behavior for most structural metals. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 67
68 SN CURVE REPRESENTATION AND APPROXIMATIONS Actual fatigue data from either specimens or parts should be used in design, if possible. Oftentimes this information is not available and must either be generated or approximations of SN behavior must be made. Common reasonable SN median fatigue life curves based upon straightline loglog approximations are shown. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 68
69 Common Reasonable SN Approximations Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 69
70 SN CURVE REPRESENTATION AND APPROXIMATIONS (CONTINUED) Basquin suggested a loglog straight line SN relationship such that S a or S Nf = A (N f ) B S a is an applied alternating stress S Nf is the fully reversed, R = 1, fatigue strength at N f cycles A is the coefficient and represents the value of S a or S Nf at one cycle B is the slope of the loglog SN curve Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 70
71 SN CURVE REPRESENTATION AND APPROXIMATIONS (CONTINUED) One approximate representation of SN curve is a trislope model with one slope between one cycle and 10 3 cycles, one between 10 3 and 10 6 or 10 8 cycles, and another slope after 10 6 or 10 8 cycles. The trislope model indicates a fatigue limit does not exist, which may be the case for service variable amplitude loading. The trislope model exists in some design codes such as for gears and welds. The trislope model could also have the third, or longlife, slope be horizontal after 10 6 or 10 8 cycles. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 71
72 SN CURVE REPRESENTATION AND APPROXIMATIONS (CONTINUED) Other approximation models assume one sloping straight line from one cycle to 10 6, 10 7, or 10 8 cycles followed by a horizontal line or another sloped line. The intercept, A, at N f = 1 could be chosen as the ultimate tensile strength, S u, the true fracture strength, f, or fatigue strength coefficient, f '. Basquin s equation using f ' is based on reversals, 2N f, rather than cycles, N f. S a or S Nf = f ' (2N f ) b Values of the f ', and b, defined as the fatigue strength coefficient and the fatigue strength exponent respectively, are given in Table A.2 for a few selected engineering alloys. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 72
73 Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 73
74 SN CURVE REPRESENTATION AND APPROXIMATIONS (CONTINUED) The slope, B, depends upon many factors and for unnotched parts could vary from about 0.05 to 0.2. For example, the varying slope can be indicated by using surface effects with S f taken from Fig Surface effects are dominant at long fatigue lives and less significant at short lives with convergence of the SN curves at S u at N f = 1. This gives different values of slope B for each surface condition. The convergence at N f = 1 is reasonable because surface finish does not have an appreciable affect on monotonic properties for most smooth metal specimens. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 74
75 SN CURVE REPRESENTATION AND APPROXIMATIONS (CONTINUED) Oftentimes the slope, B, for smooth unnotched specimens is about This suggests that for unnotched specimens the fatigue life is approximately inversely proportional to the 10 th power of alternating stress. Thus, a 10% increase or decrease in alternating stress will cause about a factor of three decrease or increase, respectively, in fatigue life. For notched parts the slope of the SN curve on logarithmic scales is steeper yielding more extreme changes. Thus, even small changes in applied alternating stress can have a significant effect on fatigue life. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 75
76 Constant Fatigue Life Diagrams Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 76
77 SN CURVE REPRESENTATION AND APPROXIMATIONS (CONTINUED) The following equations provide information to determine estimates of allowable S and S m for a given fatigue life of unnotched parts. and S Nf = A (N f ) B S a /S Nf + S m /S u = 1 or S a /S Nf + S m / f = 1 Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 77
78 SUMMARY AND DOS AND DON TS IN DESIGN Test systems are available to perform fatigue and durability tests for almost every conceivable situation from a small highly polished laboratory specimen to that of a large scale complex structure. The fatigue limit under constant amplitude loading conditions occurs for a few metals (notably low and medium strength steels), but under inservice variable amplitude loading with corrosive, temperature, or other environmental conditions, the fatigue limit is rare. The fully reversed rotating beam smooth specimen fatigue strength, S f, at 10 6 to 10 8 cycles ranges from about 0.25 to 0.65 times the ultimate tensile strength, S u. For real parts, this can vary from about 0.01 to 0.7. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 78
79 SUMMARY AND DOS AND DON TS IN DESIGN (CONT D) Yielding, finite or long life, and mean stress effects can be approximated with the following models: Yielding: S a /S y ' + S m /S y = 1 Basquin equation: S Nf = A (N f ) B Mean stress finite life S a /S Nf +S m /S u = 1 or S a /S Nf +S m / f = 1 Mean stress long life S a /S f + S m /S u = 1 or S a /S f + S m / f = 1 Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 79
80 SUMMARY AND DOS AND DON TS IN DESIGN (CONT D) Do consider that the fully reversed fatigue strength, S f, at 10 6 to 10 8 cycles for components can vary from about 1 to 70 percent of the ultimate tensile strength. Do note that cleaner metals, and generally smaller grain size for ambient temperature, have better fatigue resistance. Do recognize that frequency effects are generally small only when corrosion, temperature or other aggressive environmental effects are absent. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 80
81 SUMMARY AND DOS AND DON TS IN DESIGN (CONT D) Do consider that surface finish can have a substantial influence on fatigue resistance particularly at longer lives. Don't neglect the advantages of compressive mean or compressive residual stresses in improving fatigue life and the detrimental effect of tensile mean or tensile residual stresses in decreasing fatigue life. Do attempt to use actual fatigue data in design, but if this is not possible or reasonable, approximate estimates of median fatigue behavior can be made. Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 81
82 EXAMPLE PROBLEM USING STRESSLIFE (SN) APPROACH Ali FatemiUniversity of Toledo All Rights Reserved Chapter 4Fatigue Tests & SN Approach 82
STRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationFATIGUE FROM VARIABLE AMPLITUDE LOADING. Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1
FATIGUE FROM VARIABLE AMPLITUDE LOADING Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1 FATIGUE FROM VARIABLE AMPLITUDE LOADING SPECTRUM LOADS AND CUMULATIVE
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationExperiment: Fatigue Testing
Experiment: Fatigue Testing Objectives  To demonstrate the use of the Instron servohydraulic testing machine for testing specimens subjected to cyclic (fatigue) loadings.  To analytically approximate
More informationRESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE
RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE Ali FatemiUniversity of Toledo All Rights Reserved Chapter 8 Residual Stresses & Their Effects 1 RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE
More informationME311 Machine Design
ME Machine Design Lecture 5: FullyReversing Fatigue and the SN Diagram W Dornfeld Oct26 Fairfield University School of Engineering Discovering Fatigue With the Industrial Revolution came the steam engine
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationFatigue Failure Due to Variable Loading
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationFatigue of Metals Copper Alloys. Samuli Heikkinen 26.6.2003
Fatigue of Metals Copper Alloys Samuli Heikkinen 26.6.2003 T 70 C Temperature Profile of HDS Structure Stress amplitude 220 MPa Stress Profile of HDS Structure CLIC Number of Cycles f = 100 Hz 24 hours
More informationEffects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 4140 Steel
Paper 281434 Effects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 414 Steel Copyright 28 SAE International Nisha Cyril and Ali Fatemi The University
More informationPOWER SCREWS (ACME THREAD) DESIGN
POWER SCREWS (ACME THREAD) DESIGN There are at least three types of power screw threads: the square thread, the Acme thread, and the buttress thread. Of these, the square and buttress threads are the most
More informationMIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE
MIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE Introduction In this experiment, the finite life fatigue behavior of a smooth cylindrical specimen as shown in Figure 1 will be studied in
More informationLecture Slides. Chapter 8. Screws, Fasteners, and the Design of Nonpermanent Joints
Lecture Slides Chapter 8 Screws, Fasteners, and the Design of Nonpermanent Joints The McGrawHill Companies 2012 Chapter Outline Reasons for Nonpermanent Fasteners Field assembly Disassembly Maintenance
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationChapter 12 Elasticity
If I have seen further than other men, it is because I stood on the shoulders of giants. Isaac Newton 12.1 The Atomic Nature of Elasticity Elasticity is that property of a body by which it experiences
More informationLecture Slides. Chapter 10. Mechanical Springs
Lecture Slides Chapter 10 Mechanical Springs The McGrawHill Companies 2012 Chapter Outline Mechanical Springs Exert Force Provide flexibility Store or absorb energy Helical Spring Helical coil spring
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationNorth American Stainless
North American Stainless Flat Products Stainless Steel Sheet T409 INTRODUCTION NAS 409 is an 11% chromium, stabilized ferritic stainless steel. It is not as resistant to corrosion or hightemperature oxidation
More informationMaterial data sheet. EOS CobaltChrome MP1. Description
EOS CobaltChrome MP1 EOS CobaltChrome MP1 is a cobaltchromemolybdenumbased superalloy powder which has been optimized especially for processing on EOSINT M systems. This document provides information
More informationRolling  Introductory concepts
Rolling  Introductory concepts R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 8 Table of Contents 1. Rolling 
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationStructures and Stiffness
Structures and Stiffness ENGR 10 Introduction to Engineering Ken Youssefi/Thalia Anagnos Engineering 10, SJSU 1 Wind Turbine Structure The Goal The support structure should be optimized for weight and
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationFATIGUE CONSIDERATION IN DESIGN
FATIGUE CONSIDERATION IN DESIGN OBJECTIVES AND SCOPE In this module we will be discussing on design aspects related to fatigue failure, an important mode of failure in engineering components. Fatigue failure
More informationThere are as many reasons to test metals as there are metals:
Testing Their Mettle Metals testing procedures ensure quality in raw materials and finished products BY BILL O NEIL, ADRIAN RIDDICK, FRANK LIO, PAUL KING, CHRIS WILSON, AND PATTY HARTZELL There are as
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationChapter 7: Fatigue and Impact
Chapter 7: Fatigue and Impact All machine and structural designs are problems in fatigue because the forces of Nature are always at work and each object must respond in some fashion. Carl Osgood, Fatigue
More informationFatigue Resistance of High Strength Bolts with Large Diameters
1 Fatigue Resistance of High Strength Bolts with Large Diameters Prof. Peter Schaumann; Dipl.Ing. Frithjof Marten Leibniz Universitaet Hannover Institute for Steel Construction Hannover, Germany schaumann@stahl.unihannover.de;
More informationLecture slides on rolling By: Dr H N Dhakal Lecturer in Mechanical and Marine Engineering, School of Engineering, University of Plymouth
Lecture slides on rolling By: Dr H N Dhakal Lecturer in Mechanical and Marine Engineering, School of Engineering, University of Plymouth Bulk deformation forming (rolling) Rolling is the process of reducing
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationDESIGN TO PREVENT FATIGUE
W H I T E P A P E R DESIGN TO PREVENT FATIGUE Overview In 1954, two crashes involving the world s first commercial airliner, the de Havilland Comet, brought the words metal fatigue to newspaper headlines
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationMaterials Issues in Fatigue and Fracture
Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view
More informationMechanics of MaterialsSteel
Mechanics of MaterialsSteel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationMaterial data sheet. EOS Aluminium AlSi10Mg for EOSINT M 270. Description
EOS Aluminium AlSi10Mg for EOSINT M 270 EOS Aluminium AlSi10Mg is an aluminium alloy in fine powder form which has been specially optimised for processing on EOSINT M systems This document provides information
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationChapter 5: Tool Dynamometers
Chapter 5: Tool Dynamometers LEARNING OBJECTIVES Different types of transducers used in Dynamometers Design Requirements Types of Dynamometers 
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationOptimum proportions for the design of suspension bridge
Journal of Civil Engineering (IEB), 34 (1) (26) 114 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering
More informationThe Mechanical Behavior and Buckling Failure of SharpNotched SUS 304 Stainless Steel Tubes Subjected to Pure Bending Creep
The Mechanical Behavior and Buckling Failure of SharpNotched SUS 304 Stainless Steel Tubes Subjected to Pure Bending Creep * KuoLong Lee 1) and *WenFung Pan 2) 1) Department of Innovative Design and
More informationTubing Data. Contents. Tubing Selection. Tubing Handling. Tubing Material. Tubing Outside Diameter Hardness. Tubing Wall Thickness
www.swagelok.com Tubing Data Contents Tubing Selection... 1 Tubing Handling.... 1 Gas Service... 2 Tubing Installation.... 2 Suggested Allowable Working Pressure Tables Carbon Steel Tubing... 3 Stainless
More informationExperiment: Mechanical Testing Impact & Hardness Testing
Experiment: Mechanical Testing Impact & Hardness Testing Objective The main objective of this experiment is to introduce two important basic mechanical property tests; hardness (using Rockwell testing)
More informationCORRELATION BETWEEN HARDNESS AND TENSILE PROPERTIES IN ULTRAHIGH STRENGTH DUAL PHASE STEELS SHORT COMMUNICATION
155 CORRELATION BETWEEN HARDNESS AND TENSILE PROPERTIES IN ULTRAHIGH STRENGTH DUAL PHASE STEELS SHORT COMMUNICATION Martin Gaško 1,*, Gejza Rosenberg 1 1 Institute of materials research, Slovak Academy
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationEML 5526 FEA Project 1 Alexander, Dylan. Project 1 Finite Element Analysis and Design of a Plane Truss
Problem Statement: Project 1 Finite Element Analysis and Design of a Plane Truss The plane truss in Figure 1 is analyzed using finite element analysis (FEA) for three load cases: A) Axial load: 10,000
More informationAFRLRXWPTP20114376
AFRLRXWPTP20114376 HIGH CYCLE FATIGUE PROPERTIES OF HAYNES 230 BEFORE AND AFTER EXPOSURE TO ELEVATED TEMPERATURES (PREPRINT) R.J. Morrissey and R. John Metals Branch Metals, Ceramics & Nondestructive
More informationIMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH
ENGINEERING PAPER 524408 IMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March
More informationMaterial data sheet. EOS Aluminium AlSi10Mg. Description
EOS Aluminium AlSi10Mg EOS Aluminium AlSi10Mg is an aluminium alloy in fine powder form which has been specially optimised for processing on EOSINT M systems This document provides information and data
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationMaterial data sheet. EOS NickelAlloy IN625. Description
EOS NickelAlloy IN625 EOS NickelAlloy IN625 is a heat and corrosion resistant nickel alloy powder which has been optimized especially for processing on EOSINT M systems. This document provides information
More informationUnderstanding Fatigue
by D.P. DeLuca United Technologies Pratt & Whitney Understanding Fatigue In the gas turbine industry, whether it is in the power generation or propulsion sectors, durability is perhaps the most significant
More informationStructural materials Characteristics, testing, strength evaluation
Budapest University of Technology and Economics Department of Mechanics and Materials of Structures English courses General course /2013 Fundamentals of Structures BMEEPSTG201 Lecture no. 3: Structural
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationHardened Concrete. Lecture No. 14
Hardened Concrete Lecture No. 14 Strength of Concrete Strength of concrete is commonly considered its most valuable property, although in many practical cases, other characteristics, such as durability
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More information1.Adapted from Gordon, J.E., Structures or why things don t fall down, Da Capo Press, Inc., New York, N.Y., 1978, Chapter 15.
Lecture 4: Cyclic loading and fatigue Safe working life: 1 All structures will be broken or destroyed in the end just as all people will die in the end. It is the purpose of medicine and engineering to
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationHigh carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance
Data Sheet: A2.2 High carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance General description Steel is generally classified as high carbon steel if the nominal
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationSHORE A DUROMETER AND ENGINEERING PROPERTIES
SHORE A DUROMETER AND ENGINEERING PROPERTIES Written by D.L. Hertz, Jr. and A.C. Farinella Presented at the Fall Technical Meeting of The New York Rubber Group Thursday, September 4, 1998 by D.L. Hertz,
More informationFatigue Life Estimates Using Goodman Diagrams
Fatigue Life Estimates Using Goodman Diagrams by Robert Stone The purpose of this paper is to review the proper methods by which spring manufacturers should estimate the fatigue life of a helical compression
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationSTAVAX SUPREME. Stainless tool steel
STAVAX SUPREME Stainless tool steel General Demands placed on plastic mould tooling are increasing. Such conditions require mould steels that possess a unique combination of toughness, corrosion resistance
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationINFLUENCE OF SHOT PEENING ON CHROMIUM ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH
INFLUENCE OF SHOT PEENING ON CHROMIUM ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH *Voorwald, H. J. C., Silva, M. P., Costa, M. Y. P., a Pigatin, L. W., Marques, B. M. F. Fatigue and Aeronautic Research
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationHighly flexible couplings
Construction and operation 8.03.00 Instructions for installation 8.03.00 Types of stress 8.04.00 Diagrams for static deformation of the coupling ring 8.05.00 Coupling size 8.07.00 Examples of combinations
More informationOptimising plate girder design
Optimising plate girder design NSCC29 R. Abspoel 1 1 Division of structural engineering, Delft University of Technology, Delft, The Netherlands ABSTRACT: In the design of steel plate girders a high degree
More information